Effect of severe plastic deformation on mechanical and ... ... EffEct of SEvErE plaStIc dEforMatIon
Embed Size (px)
Transcript of Effect of severe plastic deformation on mechanical and ... ... EffEct of SEvErE plaStIc dEforMatIon
EffEct of SEvErE plaStIc dEforMatIon on MEchanIcal and fatIguE BEhavIor of MEdIuM-c ShEEt StEEl
S. rusza,*, o. hilšera, v. ochodeka, l. Čížekb, M. Krausb, v. Marešc, a. grajcard, J. Šveca
a* VSB – Technical University of Ostrava, Department of Mechanical Technology, Faculty of Mechanical Engineering, Ostrava – Poruba, Czech Republic
b VSB – Technical University of Ostrava, Department of Materials Engineering, Faculty of Metallurgy and Materials Engineering, Ostrava – Poruba, Czech Republic
c CPIT VSB – Technical University of Ostrava, Ostrava – Poruba, Czech Republic d Silesian University of Technology, Department of Engineering Materials and Biomaterials, Gliwice, Poland
(Received 10 September 2019; accepted 14 February 2020)
The DRECE method belongs to the severe plastic deformation (SPD) processes used for the refinement of sheet metal elements. A forming device used in this method is currently being installed in the workplace in the Centre of Advanced Innovation Technologies, VSB Technical University of Ostrava. In the present work the structural characteristics and fracture morphology of Ck55 carbon steel after the application of the DRECE method with a forming tool angle of 118° are presented. The microstructure results are linked to selected mechanical properties. The tensile, hardness, and fatigue tests are performed. The methodology of non-destructive residual stresses measurement in the carbon steel after the extrusion and application of tensile tests on small samples are important for their use in technical practice. The paper presents the original results of selected properties after the application of the DRECE method on Ck55 steel, which will be used in the future to assess the application of the DRECE method and to determine other directions of the processing of ferrous alloys and steels.
Keywords: Severe plastic deformation; DRECE method; Ck55 steel; Grain refinement; Mechanical properties; Residual stress
*Corresponding author: email@example.com
Journal of Mining and Metal lurgy, Section B: Metal lurgy
New technologies which use the high deformation for obtaining the fine-grained structures are intensively studied by many authors [1, 2]. This research is concerned with the whole production of ultrafine-grained (UFG) materials using Severe Plastic Deformation (SPD). Several types of the SPD technologies serving for the production of the UFG metals were already developed at the beginning of the 1990’s as the following ones: ECAP (Equal Channel Angular Pressing), DCAP (Dissimilar Channel Angular Pressing), CONFORM (Continual Forming), HPT (High Pressure Torsion), CCDC (Cyclic Channel Die Compression), ARB (Accumulative Roll Bonding), and CGP (Constrain Groove Pressing) [3- 5]. One of them is a new type of method called DRECE (Dual Rolls Equal Channel Extrusion) designed for obtaining UFG structures in sheets and rods . The performance and applications of
nanostructured materials produced by severe plastic deformation is presented in . Research areas of the SPD processes as ECAP and the DRECE method are intensively developed [8, 9]. The effectiveness of this method is evaluated by the use of different simulations [10-12]. Appropriate adjustments of the forming tool have been designed to achieve a higher intensity of deformation. It allows obtaining the UFG structure. With the use of the simulation  the SPD is predicted to increase the intensity of deformation after 5 – 6 passes to a value max = 3.5, which is a region of medium deformation levels. The investigation of a new shear deformation method for the production of nanostructures in low-carbon steel was analysed by Raab et al. . The functionality of the forming device with a new DRECE method by the use of the SPD process has been verified, especially in non-ferrous metals and mild steels. Experimental works on low carbon steels are given in works [14- 17]. Cu and brass alloys [18, 19] and other non-
J. Min. Metall. Sect. B-Metall., 56 (2) B (2020) 161 - 170
ferrous metals [20, 21] are very often subjected to this advanced production method.
The aim of the present paper is to analyse the possibilities of the DRECE method application for strengthening the medium-C sheet steel and to find relationships between structural details and mechanical and fatigue properties.
2. Material and procedures
The study material was a cold-rolled metal sheet of medium-C steel (Ck55 grade). The chemical composition is shown in Table 1.
The strip sheet with the dimensions 58 x 2 x 1000 mm and 2000 mm length was used for the study. The sheets were extruded through the forming equipment with the DRECE method. The DRECE method is similar to the Dissimilar Channel Angular Pressing process (DCAP). The scheme of the DRECE method is shown in Figure 1 and a forming device for the extrusion of strip sheets is shown in Figure 2.
The equipment consists of the following main parts: a Nord (SK7382/22VX2WD-71S/4TF) gear with an electric drive, a disc clutch, a feed roller, and pressure rollers with the regulation of thrust, and a forming tool made of the special steel Dievar (AISI H13). A strip of the sheet is fed into the working space and it is pushed by the feed roller with the help of pressure rollers through the forming tool without a change of its cross section .
Mechanical properties (yield strength Rp0.2, ultimate tensile strength Rm, ductility A80) on a test-stand LFV 100-HM produced by the Swiss company Walter + Bai ag (see Figure 3a) and hardness HV10 using a hardness tester HPO 250 were evaluated in the initial state and
after the forming process. The tensile tests were performed according to the ISO 6892 - 1 using standard test-pieces according to Annex D. The sample was cut at the longitudinal direction of the sheet deformation. Five samples were used for each condition. The average values and standard deviations were calculated.
The fatigue strength was tested using a test-stand LFV 100-HM (Figure 3a) with specially prepared samples (Figure 3b) to determine the site of fatigue fracture initiation at the constriction place. An alternating load with a frequency of 40 kHz was used.
The tensile test on small samples was evaluated in the initial state and after the forming process to assess the possibility of anisotropic properties occurrence after the SPD process. The schematic representation of the sheet metal with the indication of the places for removal samples and its size are shown in Figure 4a and 4b. As it can be seen, the sample was cut at the longitudinal and perpendicular directions of the sheet deformation.
The investigations were completed by the metallographic evaluation of the microstructure at successive stages of the forming process. Light microscopy (Neophot 2) was employed to reveal the microstructure of the steels using the bright field technique. Conventional metallographic techniques (mechanical grinding with SiC paper up to 2000 grid and polishing with a diamond paste) for the samples’ preparation followed by Nital etching were applied. The fracture surfaces of the samples after the fatigue tests were analyzed. The analysis was done by using ASPEX PSEM EXPLORER scanning electron microscope.
To assess the effect of the SPD process on the generation and redistribution of residual stresses the magnetoelastic method based on the Barkhausen noise was used. The precise knowledge of the level
S. Rusz et al. / J. Min. Metall. Sect. B-Metall., 56 (2) B (2020) 161 - 170 162
Figure 1. Scheme of the DRECE method
Chemical composition (weight %) C Mn Si P S Cr Ni Mo Fe
0.52-0.6 0.6-0.9 max. 0.4 max. 0.04 max. 0,04 max. 0.25 max. 0.3 max. 0.1 base
Table 1. Chemical composition of medium-C steel according to the standard
Figure 2. Forming device for the extrusion of strip sheets
and distribution of residual stresses are crucial for the successful application of the materials in the industry.
3. results and discussion 3.1. Hardness and mechanical properties
A schematic illustration of the sampling used to monitor the evolution of the reinforcement after the DRECE process depending on the position in the sheet sample is shown in Figure 5. The measure of the strengthening was assessed by applying HV10 hardness.
The results of the HV10 hardness measurement depending on the position in the sheet metal and number of passes are shown in Figure 6. The hardness values represent the average of the five measurements. As can be seen, the hardness is the highest on the surface area compared to the values measured in the cross section. The hardness values increase significantly after the first passage. After further passages, the increase in hardness is slower. It is also evident from the graph that the increase in hardness of the surface layer with the increasing number of passages is greater than in the cross section, which is in accordance with the analysis of the deformation in the material volume based on the computer simulation .
The results of mechanical properties received from the tensile test and hardness test are shown in Figure 7. On the basis of the results obtained from the tensile tests, it can be stated with respect to the initial state that after the 2nd pass the yield strength Rp0,2 is increased by 118 MPa and the ultimate tensile strength Rm by 42 MPa.
At the same time, there is a slight corresponding decrease in ductility (approx. 8%). After the 6th pass through the forming tool, the yield strength increased
by 180 MPa and the ultimate tensile strength by 80 MPa relat